#------------------------------------------------------------------------------
#$Date: 2019-03-05 10:52:05 +0200 (Tue, 05 Mar 2019) $
#$Revision: 213973 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/10/48/7104847.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7104847
loop_
_publ_author_name
'Han, Lei'
'Hong, Maochun'
'Wang, Ruihu'
'Luo, Junhua'
'Lin, Zhengzhong'
'Yuan, Daqiang'
_publ_section_title
;
 A novel nonlinear optically active tubular coordination network based on
 two distinct homo-chiral helices
;
_journal_coden_ASTM              CHCOFS
_journal_issue                   20
_journal_name_full
;
 Chemical Communications (Cambridge, United Kingdom)
;
_journal_page_first              2580
_journal_page_last               2581
_journal_paper_doi               10.1039/b308007b
_journal_year                    2003
_chemical_formula_sum            'C13 H11 N O3 S Zn'
_chemical_formula_weight         326.66
_space_group_IT_number           4
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 112.091(3)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   10.9901(12)
_cell_length_b                   5.8238(7)
_cell_length_c                   12.5648(13)
_cell_measurement_reflns_used    48
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      25.08
_cell_measurement_theta_min      1.75
_cell_volume                     745.16(14)
_computing_cell_refinement       'Smart and Saznt (Siemens, 1994)'
_computing_data_collection       'Smart (Siemens, 1994)'
_computing_data_reduction        'SHELXTL (Sheldrick, 1997)'
_computing_molecular_graphics    'SHELXTL (Sheldrick, 1997)'
_computing_publication_material  'SHELXTL (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 8.192
_diffrn_measured_fraction_theta_full 0.970
_diffrn_measured_fraction_theta_max 0.970
_diffrn_measurement_device_type  'Smart CCD'
_diffrn_measurement_method       'ω scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0180
_diffrn_reflns_av_sigmaI/netI    0.0373
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            2410
_diffrn_reflns_theta_full        25.08
_diffrn_reflns_theta_max         25.08
_diffrn_reflns_theta_min         1.75
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  .
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    1.789
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  .6805
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'SADABS (Sheldrick, 1996)'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.456
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    .
_exptl_crystal_description       block
_exptl_crystal_F_000             332
_exptl_crystal_size_max          0.52
_exptl_crystal_size_mid          0.30
_exptl_crystal_size_min          0.22
_refine_diff_density_max         1.024
_refine_diff_density_min         -0.622
_refine_diff_density_rms         0.192
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.04(4)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.207
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     172
_refine_ls_number_reflns         2026
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.207
_refine_ls_R_factor_gt           0.0551
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1050P)²+1.4653P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1668
_refine_ls_wR_factor_ref         0.1815
_reflns_number_gt                1888
_reflns_number_total             2026
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            b308007b.txt
_cod_data_source_block           a
_cod_original_sg_symbol_H-M      P2(1)
_cod_database_code               7104847
#BEGIN Tags that were not found in dictionaries:
_refine_ls_r_factor_ref          0.0632
#END Tags that were not found in dictionaries
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Zn1 Zn 0.42476(9) 0.45059(19) 0.91987(7) 0.0369(3) Uani 1 1 d . . .
S1 S 0.2026(3) 1.0768(6) 0.1656(2) 0.0492(7) Uani 1 1 d . . .
O1 O 0.3350(8) 0.8526(14) 0.7736(6) 0.059(2) Uani 1 1 d . . .
O2 O 0.4298(7) 0.5176(14) 0.7686(6) 0.055(2) Uani 1 1 d . . .
O3 O 0.4774(8) 0.1349(13) 0.9504(6) 0.0549(19) Uani 1 1 d . . .
N1 N -0.2271(7) 0.9723(19) 0.1044(6) 0.0417(18) Uani 1 1 d . . .
C1 C 0.3756(10) 0.7028(19) 0.7221(8) 0.043(2) Uani 1 1 d . . .
C2 C 0.3530(9) 0.7353(17) 0.5980(7) 0.039(2) Uani 1 1 d . . .
C3 C 0.3779(10) 0.567(2) 0.5345(8) 0.046(2) Uani 1 1 d . . .
H3A H 0.4121 0.4280 0.5696 0.055 Uiso 1 1 calc R . .
C4 C 0.3537(10) 0.596(2) 0.4176(8) 0.048(2) Uani 1 1 d . . .
H4A H 0.3706 0.4775 0.3755 0.058 Uiso 1 1 calc R . .
C5 C 0.3012(9) 0.937(3) 0.5426(7) 0.047(2) Uani 1 1 d . . .
H5A H 0.2813 1.0547 0.5834 0.056 Uiso 1 1 calc R . .
C6 C 0.2782(10) 0.968(3) 0.4277(8) 0.051(2) Uani 1 1 d . . .
H6A H 0.2439 1.1073 0.3927 0.061 Uiso 1 1 calc R . .
C7 C 0.3046(8) 0.8013(19) 0.3659(7) 0.038(2) Uani 1 1 d . . .
C8 C 0.2910(9) 0.830(2) 0.2413(7) 0.050(3) Uani 1 1 d . . .
H8A H 0.2480 0.6940 0.1993 0.060 Uiso 1 1 calc R . .
H8B H 0.3786 0.8347 0.2397 0.060 Uiso 1 1 calc R . .
C9 C 0.0376(9) 1.0221(16) 0.1465(7) 0.036(2) Uani 1 1 d . . .
C10 C -0.0553(11) 1.190(2) 0.0886(8) 0.049(3) Uani 1 1 d . . .
H10A H -0.0284 1.3233 0.0626 0.059 Uiso 1 1 calc R . .
C11 C -0.1840(10) 1.161(2) 0.0703(8) 0.046(2) Uani 1 1 d . . .
H11A H -0.2437 1.2752 0.0329 0.055 Uiso 1 1 calc R . .
C12 C -0.1398(9) 0.8088(19) 0.1588(9) 0.045(2) Uani 1 1 d . . .
H12A H -0.1705 0.6760 0.1815 0.054 Uiso 1 1 calc R . .
C13 C -0.0065(10) 0.827(2) 0.1831(9) 0.046(2) Uani 1 1 d . . .
H13A H 0.0514 0.7123 0.2228 0.056 Uiso 1 1 calc R . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O3 Zn1 O3 109.67(16) 2_657 . ?
O3 Zn1 O2 120.2(4) 2_657 . ?
O3 Zn1 O2 105.5(3) . . ?
O3 Zn1 N1 108.2(3) 2_657 2_546 ?
O3 Zn1 N1 107.9(4) . 2_546 ?
O2 Zn1 N1 104.7(3) . 2_546 ?
C9 S1 C8 104.5(5) . . ?
C1 O2 Zn1 116.0(6) . . ?
Zn1 O3 Zn1 137.6(4) 2_647 . ?
C11 N1 C12 118.5(8) . . ?
C11 N1 Zn1 118.9(7) . 2_556 ?
C12 N1 Zn1 122.6(7) . 2_556 ?
O1 C1 O2 123.2(8) . . ?
O1 C1 C2 119.6(9) . . ?
O2 C1 C2 117.0(9) . . ?
C3 C2 C5 117.2(9) . . ?
C3 C2 C1 122.0(9) . . ?
C5 C2 C1 120.7(9) . . ?
C2 C3 C4 121.9(10) . . ?
C7 C4 C3 119.2(10) . . ?
C2 C5 C6 121.4(12) . . ?
C7 C6 C5 120.9(13) . . ?
C6 C7 C4 119.4(9) . . ?
C6 C7 C8 123.7(10) . . ?
C4 C7 C8 116.8(9) . . ?
C7 C8 S1 117.1(8) . . ?
C13 C9 C10 117.9(9) . . ?
C13 C9 S1 125.1(8) . . ?
C10 C9 S1 116.9(7) . . ?
C11 C10 C9 120.4(9) . . ?
N1 C11 C10 121.8(10) . . ?
N1 C12 C13 123.5(10) . . ?
C9 C13 C12 117.9(10) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Zn1 O3 1.910(7) 2_657 ?
Zn1 O3 1.922(8) . ?
Zn1 O2 1.961(6) . ?
Zn1 N1 2.081(8) 2_546 ?
S1 C9 1.766(9) . ?
S1 C8 1.795(12) . ?
O1 C1 1.263(13) . ?
O2 C1 1.264(13) . ?
O3 Zn1 1.910(7) 2_647 ?
N1 C11 1.328(15) . ?
N1 C12 1.343(13) . ?
N1 Zn1 2.081(7) 2_556 ?
C1 C2 1.496(12) . ?
C2 C3 1.356(15) . ?
C2 C5 1.375(17) . ?
C3 C4 1.402(13) . ?
C4 C7 1.370(15) . ?
C5 C6 1.380(12) . ?
C6 C7 1.344(16) . ?
C7 C8 1.525(11) . ?
C9 C13 1.378(13) . ?
C9 C10 1.405(14) . ?
C10 C11 1.356(15) . ?
C12 C13 1.383(14) . ?
